human
***TASK*** the task is to summarize an input biomedical literature in six sentences 
    ***INPUT*** the input is a biomedical literature 
    ***OUTPUT*** the output is the summary of an input biomedical literature in six sentences 
    ***DOCUMENTATION*** 
    ***EXAMPLES*** 
    Input: OBJECTIVE To evaluate the microtensile bond strengths ( μTBS ) and nanoleakage ( NL ) of three universal or multi-mode adhesives , applied with increasing solvent evaporation times . METHODS One-hundred and forty caries-free extracted third molars were divided into 20 groups for bond strength testing , according to three factors : ( 1 ) Adhesive - All-Bond Universal ( ABU , Bisco , Inc. ) , Prime&Bond Elect ( PBE , Dentsply ) , and Scotchbond Universal Adhesive ( SBU , 3 M ESPE ) ; ( 2 ) Bonding strategy - self-etch ( SE ) or etch- and -rinse ( ER ) ; and ( 3 ) Adhesive solvent evaporation time - 5s , 15s , and 25s . Two extra groups were prepared with ABU because the respective manufacturer recommends a solvent evaporation time of 10s . After restorations were constructed , specimens were stored in water ( 37 ° C/24h ) . Resin-dentin beams ( 0.8mm(2 ) ) were tested at 0.5mm/min ( μTBS ) . For NL , forty extracted molars were r and omly assigned to each of the 20 groups . Dentin disks were restored , immersed in ammoniacal silver nitrate , sectioned and processed for evaluation under a FESEM in backscattered mode . Data from μTBS were analyzed using two-way ANOVA ( adhesive vs. drying time ) for each strategy , and Tukey 's test ( α=0.05 ) . NL data were computed with non-parametric tests ( Kruskal-Wallis and Mann-Whitney tests , α=0.05 ) . RESULTS Increasing solvent evaporation time from 5s to 25s result ed in statistically higher mean μTBS for all adhesives when used in ER mode . Regarding NL , ER result ed in greater NL than SE for each of the evaporation times regardless of the adhesive used . A solvent evaporation time of 25s result ed in the lowest NL for SBU-ER . SIGNIFICANCE Residual water and /or solvent may compromise the performance of universal adhesives , which may be improved with extended evaporation times OBJECTIVE To test the influence of a hydrophobic resin coating ( HC ) on the immediate ( 24h ) and 6-month ( 6 m ) microtensile dentin bond strengths ( μTBS ) and nanoleakage ( NL ) of three universal adhesives applied in self-etch ( SE ) or in etch- and -rinse ( ER ) mode . METHODS Sixty caries-free extracted third molars were assigned to 12 experimental groups result ing from the combination of the factors " adhesive system " ( Scotchbond Universal Adhesive [ SBU ] , 3 M ESPE ; All-Bond Universal [ ABU ] , Bisco Inc. ; and G-Bond Plus [ GBP ] , GC Corporation ) ; " adhesive strategy " ( SE or ER ) ; " hydrophobic resin coating " [ HC ] ( with or without Heliobond , Ivoclar Vivadent ) ; and " storage time " ( 24h or 6 m ) . Specimens were prepared for μTBS testing - ( 24h ) half of the beams were immediately tested under tension ; and ( 6 m ) the other half was stored in distilled water ( 37 ° C ) for 6 m prior to testing . For each tooth , two beams were r and omly selected for NL evaluation for both evaluation times . Data were analyzed for each adhesive system using three-way ANOVA and Tukey 's post-hoc test ( α=0.05 ) . RESULTS μTBS : ( 24h ) : In SE mode , HC result ed in statistically greater mean μTBS for all adhesives . ( 6 m ) : When HC was not used the mean μTBS for SBU/ER , ABU/ER , GBP/ER and SBU/SE decreased significantly . NL : ( 24h ) : SBU/ER , ABU/ER and GBP/SE result ed in a significant reduction in NL when HC was applied . ( 6 m ) : No significant reduction was observed for SBU/ER or for SBU/SE regardless of the use of HC . SIGNIFICANCE The application of a hydrophobic resin coating improved the 24h and the 6 m performances of all three adhesives systems in SE mode BACKGROUND The durability of restorations bonded with one-step self-etching ( OSSE ) adhesive systems is inferior compared with that of restorations bonded with conventional adhesives . The authors conducted an 18-month r and omized clinical study to evaluate the clinical performance of two OSSE systems in noncarious cervical lesions applied as recommended or with an extra layer of hydrophobic adhesive layer after 18 months of clinical service . METHODS Thirty participants , each of whom had at least two pairs of similar-sized noncarious cervical lesions , took part in this study . The authors placed 120 restorations  , 30 in each of four groups : Clearfil S3 Bond ( Kuraray , Osaka , Japan ) ( CS ) and iBond Gluma inside ( Heraeus Kulzer , Hanau , Germany ) ( IB ) , and Clearfil S3 Bond ( CSB ) and iBond Gluma inside ( IBB ) with an extra layer of hydrophobic adhesive applied on top of them . They placed the restorations incrementally , using a resin-based composite . The authors evaluated the restorations at baseline and at 18 months following modified U.S. Public Health Service criteria . RESULTS At 18 months , the retention rate for the IB group was statistically lower than those for the CS , IBB and CSB groups . Marginal discoloration occurred in all groups and was statistically worse in the IB group . CONCLUSIONS The conversion of the iBond Gluma inside and Clearfil S3 Bond adhesive systems into two-step systems by means of applying an extra hydrophobic adhesive layer improved the clinical performance of these material s after 18 months of clinical service . CLINICAL IMPLICATION S The application of an extra hydrophobic adhesive layer over OSSE adhesive systems , layers improved the OSSE systems clinical performance , mainly in terms of retention rate PURPOSE To investigate the bonding of a new universal adhesive applied using different etching strategies on sound and caries-affected dentin of primary teeth . MATERIAL S AND METHODS Flat dentin surfaces from 50 primary molars were r and omly assigned to 10 groups according to substrate ( sound dentin [ SD ] vs caries-affected dentin [ CAD ] pH cycled for 14 days ) and bonding approach ( Scotchbond Universal Adhesive : self-etching , vs dry or wet-bonding etch- and -rinse strategies ; Adper Single Bond Plus [ two-step etch- and -rinse adhesive ] and Clearfil SE Bond [ two-step self-etching system ] as controls ) . After 24 h of water storage , bonded sticks with cross-sectional areas of 0.8 mm2 were tested for microtensile bond strength ( μTBS ) . Two sticks from each tooth were immersed in silver nitrate solution in order to evaluate nanoleakage ( NL ) with SEM . The μTBS means were analyzed using two-way ANOVA and Tukey 's tests . For NL , the Kruskal-Wallis and Mann-Whitney tests were used ( α = 0.05 ) . RESULTS The influence of the etching strategy on the bonding performance of the universal adhesive was substrate dependent . The self-etching approach result ed in lower μTBS values and higher silver nitrate uptake into hybrid layers for Scotchbond Universal Adhesive on SD , while no difference among experimental groups was observed in CAD . CONCLUSION It is preferable to use the universal adhesive following either a dry- or wet-bonding etch- and -rinse approach on both sound and caries-affected primary dentin 
    Output:
    
agent
The meta- analysis demonstrated that the etch- and -rinse technique significantly reduced the nanoleakage of the Peak Universal and G-Bond Plus adhesives , whereas the self-etch mode reduced the nanoleakage of All-Bond Universal .
In comparison , the etching technique did not significantly alter the nanoleakage of either Prime&Bond Elect or Scotchbond Universal which was characterized by the smallest nanoleakage .
CONCLUSIONS Etching modes significantly , in various ways , influence the nanoleakage of universal adhesives .
CLINICAL SIGNIFICANCE Contrary to the drive to simplify bonding technologies , an appreciation of their adhesive components and how these perform according to bonding technique could yield a knowledge-based practical approach that ultimately improves the longevity of direct composite restorations
***TASK*** the task is to summarize an input biomedical literature in six sentences 
    ***INPUT*** the input is a biomedical literature 
    ***OUTPUT*** the output is the summary of an input biomedical literature in six sentences 
    ***DOCUMENTATION*** 
    ***EXAMPLES*** 
    Input: OBJECTIVE To evaluate the microtensile bond strengths ( μTBS ) and nanoleakage ( NL ) of three universal or multi-mode adhesives , applied with increasing solvent evaporation times . METHODS One-hundred and forty caries-free extracted third molars were divided into 20 groups for bond strength testing , according to three factors : ( 1 ) Adhesive - All-Bond Universal ( ABU , Bisco , Inc. ) , Prime&Bond Elect ( PBE , Dentsply ) , and Scotchbond Universal Adhesive ( SBU , 3 M ESPE ) ; ( 2 ) Bonding strategy - self-etch ( SE ) or etch- and -rinse ( ER ) ; and ( 3 ) Adhesive solvent evaporation time - 5s , 15s , and 25s . Two extra groups were prepared with ABU because the respective manufacturer recommends a solvent evaporation time of 10s . After restorations were constructed , specimens were stored in water ( 37 ° C/24h ) . Resin-dentin beams ( 0.8mm(2 ) ) were tested at 0.5mm/min ( μTBS ) . For NL , forty extracted molars were r and omly assigned to each of the 20 groups . Dentin disks were restored , immersed in ammoniacal silver nitrate , sectioned and processed for evaluation under a FESEM in backscattered mode . Data from μTBS were analyzed using two-way ANOVA ( adhesive vs. drying time ) for each strategy , and Tukey 's test ( α=0.05 ) . NL data were computed with non-parametric tests ( Kruskal-Wallis and Mann-Whitney tests , α=0.05 ) . RESULTS Increasing solvent evaporation time from 5s to 25s result ed in statistically higher mean μTBS for all adhesives when used in ER mode . Regarding NL , ER result ed in greater NL than SE for each of the evaporation times regardless of the adhesive used . A solvent evaporation time of 25s result ed in the lowest NL for SBU-ER . SIGNIFICANCE Residual water and /or solvent may compromise the performance of universal adhesives , which may be improved with extended evaporation times OBJECTIVE To test the influence of a hydrophobic resin coating ( HC ) on the immediate ( 24h ) and 6-month ( 6 m ) microtensile dentin bond strengths ( μTBS ) and nanoleakage ( NL ) of three universal adhesives applied in self-etch ( SE ) or in etch- and -rinse ( ER ) mode . METHODS Sixty caries-free extracted third molars were assigned to 12 experimental groups result ing from the combination of the factors " adhesive system " ( Scotchbond Universal Adhesive [ SBU ] , 3 M ESPE ; All-Bond Universal [ ABU ] , Bisco Inc. ; and G-Bond Plus [ GBP ] , GC Corporation ) ; " adhesive strategy " ( SE or ER ) ; " hydrophobic resin coating " [ HC ] ( with or without Heliobond , Ivoclar Vivadent ) ; and " storage time " ( 24h or 6 m ) . Specimens were prepared for μTBS testing - ( 24h ) half of the beams were immediately tested under tension ; and ( 6 m ) the other half was stored in distilled water ( 37 ° C ) for 6 m prior to testing . For each tooth , two beams were r and omly selected for NL evaluation for both evaluation times . Data were analyzed for each adhesive system using three-way ANOVA and Tukey 's post-hoc test ( α=0.05 ) . RESULTS μTBS : ( 24h ) : In SE mode , HC result ed in statistically greater mean μTBS for all adhesives . ( 6 m ) : When HC was not used the mean μTBS for SBU/ER , ABU/ER , GBP/ER and SBU/SE decreased significantly . NL : ( 24h ) : SBU/ER , ABU/ER and GBP/SE result ed in a significant reduction in NL when HC was applied . ( 6 m ) : No significant reduction was observed for SBU/ER or for SBU/SE regardless of the use of HC . SIGNIFICANCE The application of a hydrophobic resin coating improved the 24h and the 6 m performances of all three adhesives systems in SE mode BACKGROUND The durability of restorations bonded with one-step self-etching ( OSSE ) adhesive systems is inferior compared with that of restorations bonded with conventional adhesives . The authors conducted an 18-month r and omized clinical study to evaluate the clinical performance of two OSSE systems in noncarious cervical lesions applied as recommended or with an extra layer of hydrophobic adhesive layer after 18 months of clinical service . METHODS Thirty participants , each of whom had at least two pairs of similar-sized noncarious cervical lesions , took part in this study . The authors placed 120 restorations  , 30 in each of four groups : Clearfil S3 Bond ( Kuraray , Osaka , Japan ) ( CS ) and iBond Gluma inside ( Heraeus Kulzer , Hanau , Germany ) ( IB ) , and Clearfil S3 Bond ( CSB ) and iBond Gluma inside ( IBB ) with an extra layer of hydrophobic adhesive applied on top of them . They placed the restorations incrementally , using a resin-based composite . The authors evaluated the restorations at baseline and at 18 months following modified U.S. Public Health Service criteria . RESULTS At 18 months , the retention rate for the IB group was statistically lower than those for the CS , IBB and CSB groups . Marginal discoloration occurred in all groups and was statistically worse in the IB group . CONCLUSIONS The conversion of the iBond Gluma inside and Clearfil S3 Bond adhesive systems into two-step systems by means of applying an extra hydrophobic adhesive layer improved the clinical performance of these material s after 18 months of clinical service . CLINICAL IMPLICATION S The application of an extra hydrophobic adhesive layer over OSSE adhesive systems , layers improved the OSSE systems clinical performance , mainly in terms of retention rate PURPOSE To investigate the bonding of a new universal adhesive applied using different etching strategies on sound and caries-affected dentin of primary teeth . MATERIAL S AND METHODS Flat dentin surfaces from 50 primary molars were r and omly assigned to 10 groups according to substrate ( sound dentin [ SD ] vs caries-affected dentin [ CAD ] pH cycled for 14 days ) and bonding approach ( Scotchbond Universal Adhesive : self-etching , vs dry or wet-bonding etch- and -rinse strategies ; Adper Single Bond Plus [ two-step etch- and -rinse adhesive ] and Clearfil SE Bond [ two-step self-etching system ] as controls ) . After 24 h of water storage , bonded sticks with cross-sectional areas of 0.8 mm2 were tested for microtensile bond strength ( μTBS ) . Two sticks from each tooth were immersed in silver nitrate solution in order to evaluate nanoleakage ( NL ) with SEM . The μTBS means were analyzed using two-way ANOVA and Tukey 's tests . For NL , the Kruskal-Wallis and Mann-Whitney tests were used ( α = 0.05 ) . RESULTS The influence of the etching strategy on the bonding performance of the universal adhesive was substrate dependent . The self-etching approach result ed in lower μTBS values and higher silver nitrate uptake into hybrid layers for Scotchbond Universal Adhesive on SD , while no difference among experimental groups was observed in CAD . CONCLUSION It is preferable to use the universal adhesive following either a dry- or wet-bonding etch- and -rinse approach on both sound and caries-affected primary dentin 
    Output:
    